Home >Documents >Numerical Modeling of Heat Transfer and Damage Evolution ... Damage Evolution Strategy Specific Heat...

# Numerical Modeling of Heat Transfer and Damage Evolution ... Damage Evolution Strategy Specific Heat...

Date post:26-Jan-2021
Category:
View:0 times
Transcript:

Dr. Peter J. Joyce

MIDN 1/C Andrew Tresansky

CAPT Joseph Watkins

Mechanical Engineering Department

Numerical Modeling of Heat Transfer and

Damage Evolution due to HEL Irradiation

Excerpt from the Proceedings of the 2012 COMSOL Conference in Boston

• Overall Objective of Research Program

 Develop and validate predictive tools relevant to laser damage of materials.

 Capture laser drilled hole evolution.

 Capture radiative/transmissive damage to remainder of structure.

Puishys, J. Joyce, P. “Damage Tolerance of Laser Irradiated Composite Sandwich Structures.” USNA, 2011.

• Current Thrust

 Develop a COMSOL Multiphysics simulation of damage and hole

evolution for isotropic materials subjected to a 1070nm laser.

 Compare to experimentally observed laser damage evolution

through a simple test material (PMMA).

and Laser Specification

 Finite Thickness Plate of Large

Plan-view Area

 DE Lab Laser Parameters:

 IPG 1070nm Nd:YAG Laser.

 Power: 110W (Measured)

 Beam Diameter: 5.5mm (Per Mfg’s

Measurements)

 M2 = 1.07

z

r

D

H

Gaussian Beam Profile

“Top Hat” Beam Profile of Equal Power for Same Beam Diameter

 

I r  I0e 8 r2

D 2

• Model Assumptions

 Laser modeled as a heat flux with a Gaussian radial distribution.

 55% incident energy absorbed, 45% of incident energy reflected

in accordance with published1 Near-Infrared Reflective

Spectroscopy (NIRS) measurements at 1070nm.

 Material changes phase directly from solid to vapor.

1: Lloyd, Christopher, “Ablation of Organic Polymeric Materials”,

Doctoral Dissertation, George Mason University

• COMSOL Model: Domain and Element Model

 Axisymmetric model (only valid for isotropic materials)

 Mapped quad elements with higher fidelity near centerline

• COMSOL Model: Boundary Conditions

Axial Symmetry

Open Boundary

• Damage Evolution Strategy

 Specific Heat modified to include latent heat of vaporization over

an experimentally determined temperature span.

 Other Material properties artificially modified after vaporization.

 Density and specific heats become that of air/vaporous material.

 Thermal conductivity becomes “extremely large” in beam direction.

 Thermal conductivity becomes “extremely small” in radial direction

• Model Parameters (Part 1):

Thermal Properties and Geometry

 PMMA Properties:

 Density (ρ): 1190 kg/m3

 Thermal Conductivity (k): 0.19 W/m2-K

 Specific Heat (Cps): 1470 J/kg-K

 Air/PMMA Vapor Properties:

 Density (ρ): 1 kg/m3

 Specific Heat (Cpv): 1000 J/kg-K

 Boundary Heat Transfer Coefficients

 Convection Coefficient (h): 25 W/m2-K

 Radiation Emmissivity Coefficient (ε): 0.85

 Thickness (H): 0.25in.

• Model Parameters (Part 2):

DSC Plot and the Latent Heat of Vaporization

 Starting Vaporization

Temperature (T1): 310°C

 Ending Vaporization

Temperature (T2): 420°C

 Latent Heat of Vaporization

(ΔH): 619.9 kJ/kg

• Simulation Results (Part 1):

Qualitative Evolution of Damage

• Simulation Results Backup:

• Simulation Results (Part 2):

Quantitative Evolution of Damage

 Largest Predicted Hole Diameter (Front Surface): 0.291 in.

 Hole Evolution Rate: 0.136 in/s.

• Experimental Results (Part 1):

Laboratory Setup and Test Plan

 Laser Power: 110W

 Specimen Thicknesses:  0.25 in.

 0.5 in.

 Experimental Procedure:

 Laser Drill Specimens for Specified Times.

 Measure Local Sample Thickness Away From Hole.

 Measure Hole Depth.

• Experimental Results (Part 2):

Depth vs. Irradiance Time for 0.25in PMMA

 Largest Predicted Hole Diameter (Front Surface): 0.298 in.

 Hole Evolution Rate: 0.116 in/s.

• Experimental Results (Part 3):

Depth vs. Irradiance Time for 0.50in PMMA

 Largest Predicted Hole Diameter (Front Surface): 0.298 in.

 Hole Evolution Rate: 0.117 in/s.

• Comparisons and Conclusions

 COMSOL Multiphysics Model:

 Burn-through Rate: 0.136 in/s

 Largest Hole Diameter: 0.291 in.

 Experimental Results:

 Burn-through Rate: 0.117 in/s

 Largest Hole Diameter: 0.298 in.

 Model Deviation from Experiment:

 20% Overprediction of Burn Rate

 2% Underprediction of Hole Diameter

• Acknowledgements

 Office of Naval Research Directed Energy Research Center

 Dr. Cody Brownell

Mechanical Engineering Department

 ENS Joseph Puishys

United States Navy

• Any Questions?

Embed Size (px)
Recommended

Documents

Documents

Documents

Documents

Documents

Documents

Documents

Documents

Documents

Documents

Documents

Documents

Documents

Documents

Documents

Documents

Documents

Documents